# 1-3.3 GRAIN-BOUNDARY SLIDING

```‫فرع السيراميك ومواد البناء‬/‫المرحلة الثالثة‬
Characteristic of Ceramic Materials/mechanical properties
1-3.3 GRAIN-BOUNDARY SLIDING
Some ceramics have an intergranular film (IGF) formed during fabrication,
often due to the addition of a sintering aid. If this phase softens at high temperature
then we get creep by grain-boundary sliding. The glass viscosity, η, which is a
function of temperature, controls the creep rate. As the temperature increases the
viscosity decreases, and this is usually represented by an empirical relation known as
the Vogel–Fulcher–Tammann (VFT) equation or sometimes simply the Fulcher
equation:
(1.18)
A, B, and T0 are constants for a particular glass. The VFT equation works very well
except at temperatures close to the glass transition temperature, Tg. There are several
mechanisms that can result in a permanent change in shape. In one mechanism the
glass is squeezed out of the boundaries during compression flowing to those under
tension. Proof of this mechanism comes from high-resolution TEM, which can be
used to directly measure the thickness, w, of the IGF. In these cases
(1.19)
Another proposed mechanism is that of dissolution and reprecipitation, which is
illustrated in Figure 1.19. Here grains dissolve in the liquid at points of high stress,
and this solute then diffuses through the liquid and precipitates at regions of low
stress. In this case the creep rate is
(1-20)
This latter mechanism is similar to what happens during liquid-phase sintering. The
requirements include the following:
- The solid must have a certain amount of solubility in the liquid.
- The liquid must wet the solid.
The composition of the IGF is important in determining overall creep behavior.
Other important aspects of the microstructure are the grain size and the volume
fraction of liquid present.
1
‫فرع السيراميك ومواد البناء‬/‫المرحلة الثالثة‬
Characteristic of Ceramic Materials/mechanical properties
FIGURE 1.19 Illustration of the dissolution–precipitation mechanism that could be operative
in ceramics containing a glassy phase at the GB.
1-3.4 TERTIARY CREEP AND CAVITATION
Tertiary creep represents the final stage of creep deformation and involves an
acceleration of the creep rate followed by failure of the component. This stage does
not occur in all ceramics, and as previously noted certain ceramics exhibit only
primary creep. Tertiary creep involves the formation of cavities that lead to crack
formation, often along grain boundaries. The cracks can propagate rapidly,
Although the nucleation of cavities does not seem to be well understood at present
it is clear that cavitations depends on microstructure. Porosity and second-phase
particles, which are sources of stress concentration, can act as nucleation sites for
cavitations and subsequent crack growth. Remember pores can be found in most
ceramics; even “pore-free” materials such as hot pressed alumina may contain small
pores. Cavitations also occur in ceramics with IGFs. Figure 1.20 shows cavity size
distribution data for two polycrystalline alumina. One is Lucalox (there is no glassy
phase) and the other is 99% pure alumina with a glassy phase. The data were
obtained using small-angle neutron scattering. For Lucalox the number of pores
increases with increasing creep strain but their size does not increase—nucleation is
the dominant process. For the alumina with a glassy phase both the number and size
of the pores increase with creep strain—we are getting both nucleation and growth.
2
‫فرع السيراميك ومواد البناء‬/‫المرحلة الثالثة‬
Characteristic of Ceramic Materials/mechanical properties
FIGURE 1.20 (a) Cavity-size distribution as a function of creep strain in alumina without a
glassy phase (Lucalox). (b) Cavity-size distribution as a function of creep strain in alumina
1-3.5 CREEP DEFORMATION MAPS
From the previous sections you can see that there are a large number of creep
mechanisms. These can be expressed by one general equation:
(1.21)
The various creep mechanisms give rise to different values of the exponents, m and
n. For a given ceramic a specific creep mechanism may dominate at certain
temperatures and stresses. This can be represented on a creep deformation map as
illustrated in Figure 1.21. These maps are based on a large amount of experimental
data.
FIGURE 1.21 (a) Schematic of creep deformation
Map for a polycrystalline ceramic.
3
‫فرع السيراميك ومواد البناء‬/‫المرحلة الثالثة‬
Characteristic of Ceramic Materials/mechanical properties
1-3.6 VISCOUS FLOW
Viscous flow is an important mechanism for permanent deformation in glasses.
Viscous flow is also a mechanism by which ceramics containing IGFs undergo creep.
So it is a characteristic that is both beneficial and deleterious, but unavoidable at high
temperature. Under most conditions oxide glasses behave as Newtonian fluids, i.e.,
the strain rate, dγ/dt, is a linear function of the applied shear stress, τ. At high stress
levels non-Newtonian behavior, which is common in polymers, may be observed in
oxide glasses.
The viscosity of a specific glass depends on temperature as shown in
Figure 1.22 Glass blowing is often performed at viscosities of ~10 MPa・s. This is at
the top end of the working range, which extends from 1 kPa・s to 10 MPa・s. If the
viscosity was at the fining temperature (~5 Pa・s) the gas would have been able to
escape easily. If the viscosity were too high the glass would not have been able to
deform in this way. There is also time dependence to the viscosity, particularly near
Tg and above. At these temperatures structural relaxation occurs.
FIGURE 1.22 Temperature dependence of Viscosity for a soda lime- silica glass.
4
```

37 cards

39 cards

63 cards

43 cards

44 cards